In this paper, we have reported a multifunctional device from graphene/TiO2/p-Si heterojunction, followed by its systematical analysis of optical response in a device under ultraviolet–visible-infrared band and transmission changes of terahertz waves in the 0.3–1.0 THz band under different bias voltages. It is found that photodetector in the “back-to-back” p-n-p energy band structure has a seriously unbalanced distribution of photogenerated carriers in the vertical direction when light is irradiated from the graphene side. So this ensures a higher optical gain of the device in the form of up to 3.6 A/W responsivities and 4 × 1013 Jones detectability under 750 nm laser irradiation. Besides, the addition of TiO2 layer in this terahertz modulator continuously widens the carrier depletion region under negative bias, thereby realizing modulation of the terahertz wave, making the modulation depth up to 23% under − 15 V bias. However, almost no change is observed in the transmission of terahertz wave when a positive bias is applied. A similar of an electronic semiconductor diode is observed that only allows the passage of terahertz wave for negative bias and blocks the positive ones.
An optoelectronic device such as a photodetector converts the light signal into an electrical signal and is widely used in optical communications, thermal imaging, environmental monitoring, biomedical imaging, etc. [1,2,3,4,5]. Terahertz (THz) broadband modulator is a key device to realize the practical application of terahertz wave in communication, imaging, sensing and other application areas [6,7,8,9,10]. Therefore, the development of a high-speed modulator that works at room temperature, small in size, and easy to process, is of great significance for the development and practicality of terahertz technology.
Recently, graphene has been employed in the field of photodetectors and terahertz modulators due to its special energy band structure and ultra-high carrier mobility [11,12,13,14,15,16]. So, graphene-based multifunctional photodetectors and terahertz modulators can overcome the above issue due to its miniaturization of electronic communication systems. Graphene-based photodetectors have been extensively studied in the past few years. Graphene/Si heterojunction has high photoelectric conversion efficiency and thus has great potential to obtain high-performance photodetectors [17,18,19,20]. However, the low optical absorption of graphene (~ 2.3% for a single layer of graphene) is responsible for low responsivity [21, 22]. The interface between Si and graphene contains a large number of surface states pinning the surface Fermi level, leading to a strong leakage current noise. Various methods have been proposed to improve the performance of graphene/silicon photodetectors, including insertion of an interfacial oxide layer, silicon waveguide integration, optical absorption layer addition, and surface plasmon enhancement [23,24,25,26,27,28,29].
In the case of graphene-based terahertz modulators, both optical pump and external voltage bias can be used as excitation signals. To perform all-optical modulation of terahertz waves, Wen et al.  proposed a modulator where a layer of graphene is placed on a germanium substrate. When the sample is irradiated with a 1550 nm communication wavelength laser, the terahertz transmission intensity sharply dropped along with the increase in laser power. The modulation depth reaches 94% in the frequency range of 0.25–1 THz. Professor Sensale et al.  used a graphene-based field effect transistor (GFET), where 92 nm SiO2 is used as a dielectric layer of terahertz modulator with a modulation depth of 15% and modulation rate of 18 Kb/s. This type of THz wave wide-band modulator completely uses electron and hole concentration changes in the graphene film for the control attenuation of terahertz wave energy. After that, aluminum oxide Al2O3, YIG, and other materials [32,33,34] can effectively reduce the Coulomb scattering and cavity effect of graphene due to their high dielectric constant and thus are used as the dielectric layer of GFET terahertz wave modulator.
In this study, graphene/TiO2/p-Si trilayer heterojunction is fabricated to design a photodetector and a broadband THz wave modulator. Moreover, our designed device can also work as a diode for terahertz waves that can only pass the current of negative bias and blocks the positive one.
The prototype of a multifunctional photodetector and THz modulator based on graphene/TiO2/p-Si heterojunction is shown in Fig. 1. The TiO2 film is deposited on the p-Si substrate (500-μm-thick, resistivity ρ ~ 1–10 Ω cm), using the low-temperature hydrothermal method. The cleaned silicon substrate was immersed into 0.1 M TiCl4 aqueous solution at 343 K for one hour to obtain about 10-nm-thick TiO2 film. A single layer of graphene is grown on the copper substrate by chemical vapor deposition , then spin-coated with PMMA, and immersed into 1 mol/L FeCl3 solution for 90 min to remove the copper background. After that, the TiO2/p-Si substrate was used to pick up the PMMA-coated monolayer graphene and then dry it to remove PMMA , and get graphene/TiO2/p-Si trilayer heterojunction, the PMMA-coated graphene/TiO2/p-Si substrare is immersed in acetone solution. The photoresponses of graphene/TiO2/p-Si heterojunction, such as photogenerated current and time-dependent characteristics, were measured on a monochromator (Zolix, Omni-λ 300i), which use order sorting filters to provide white and monochromatic light. The I–V curves and I–t curves of the graphene/TiO2/p-Si heterojunction under light illumination were measured by a SourceMeter (Keithley 2601B). The terahertz wave transmission was measured by a Fico THz time domain system (Zomega Terahertz Corporation).
Results and discussion
The dark current of the device and the photocurrent when excited by white light changes with the bias voltage, and change in current with a voltage of 2 Hz white light is shown in Fig. 2a. From Fig. 2a, we can see that the device has an obvious rectifying effect. The positive direction of applied voltage is from the silicon to graphene side, which indicates that the main built-in electric field of the device is due to silicon-titanium oxide junction. On the other hand, the built-in electric field introduced by weak p-type graphene [37, 38] and weak n-type TiO2 can be ignored. Under the negative bias voltage, the built-in electric field is further enhanced by the external bias voltage. When light is irradiated from the graphene side, a large number of photogenerated carriers are collected by the graphene which is quickly transmitted out. This results in an imbalance between the photo-generated carriers on the graphene and silicon side, which consequences in a strong optical guide gain under high bias. When 2 Hz white light is applied, the current coincides with the dark current (no light) and coincides with the photocurrent (when light is applied), which shows that the device has a high response speed and good repeatability. As shown in Fig. 2b, graphene/TiO2/p-Si has an obvious photoelectric response in the range of 350–1050 nm wavelength at a bias of − 2 V. Furthermore, it can be seen from Fig. 2 that the dark current of the device does not significantly change under different wavelengths of laser irradiation. However, the dark current slightly increases along with the increase in time. This is caused by the heat loss when the device is working. When the working time of the device is extended, a local temperature is raised, which causes an increase in leakage of current. Photocurrent of the device obviously changes under different light waves (350–1050 nm). The photoresponse currents (Ion − Ioff) at 350, 55, 750, 950, and 1050 nm are 126.29, 213.35, 189.67, 335.93, and 102.46 μA, respectively.
The spectra-dependent of responsivity (R), external quantum efficiency (EQE), and detectivity (D*) of the heterojunction are shown in Fig. 3a, b. The performance of photodetectors can be evaluated from the R, EQE and D* parameters. Responsivity (R) is defined as R = (Ion − Ioff)/Pin, where Ion, Ioff and Pin are photocurrents, dark current, and incident light power. External quantum efficiency (EQE) is the number of electron–hole pairs excited by the unit incident photon, which reflects the sensitivity of photodetectors to photons and can be calculated as EQE = Rhc/λ. Here h, c and λ are Plank’s constant, elementary charge, and wavelength of incident light, respectively. Detectivity (D*) can be expressed as D* = R/(2qId/A)1/2, where Id is the dark current and A is an active area (0.5 cm2). The highest responsivity and EQE of 3.6 A/W and 6001% are observed under light with 0.417 mW/cm2 intensity and 750 nm wavelength. Detectivity is 4 × 1013 Jones at 750 nm light, which is about 520 times higher than the graphene/Si photodetector . Light is irradiated from the graphene side, and the carriers excited by the short-wavelength are near the TiO2 side. At this time, the electrons are quickly collected by the graphene under the negative bias voltage. However, holes could not travel a long distance on the silicon side, cause charge recombination, and reduce the photoresponse of the device. Besides, insufficient absorption of long-wavelength light by Si can also reduce the photoresponse of the device. It is found that excitation light of about 750 nm wavelength can be completely absorbed by Si, and the distribution of photogenerated carriers in the thickness direction of the device is relatively uniform, so the best responsivity is obtained.
The THz wave transmittance of THz wave of the graphene/TiO2/p-Si heterojunction in the range of 0.3–1 THz is shown in Fig. 4a. It can be seen from Fig. 4a that when a positive bias voltage of 5 V and 10 V is applied, the transmittance of the THz wave hardly changes compared to 0 V. When negative bias voltages of − 10 V, − 15 V, and − 20 V are applied, the THz wave transmittance significantly changed. The direction of the applied negative bias electric field is the same as the direction of a built-in electric field of p-Si and TiO2. As the negative bias voltage increases, the space charge region widens, and the device gradually becomes fully depleted. Meanwhile, there is no carrier accumulation inside the device, the carriers move along the external circuit, and transmission of the terahertz wave increases. The modulation depth is an important performance parameter of terahertz modulators, which can be calculated by (Texcitation − Tno excitation)/Tno excitation, where the Texcitation and Tno excitation represent the intensity of THz transmission with and without photoexcitation, respectively. The variation in modulation depth of the device under different bias voltages in the range of 0.3–1.0 THz is calculated, and the result is shown in Fig. 4b. It can be seen from Fig. 4b that when 5 V and 10 V are applied, the modulation depth is approximately zero. The modulation depth is about 23% at − 15 V. While at − 20 V, the modulation depth slightly decreased to about 22.6%. The reason behind this is the use of extremely high voltage, where the device breaks down in the reverse region and the current increases. Continuing to increase the voltage will not further broaden the space charge layer to increase THz transmission, but will increase the temperature of the device and increase the carrier concentration due to the thermal effect, caused by the increase in current. This decreases terahertz wave and resulting in the decrease of modulation depth.
Time-domain signals of graphene/TiO2/p-Si THz modulator with various bias voltages are plotted in Fig. 5a. We can see from the time-domain graph when a positive gate voltage is applied almost coincides with the graph when 0 V is applied. When a negative bias is applied, the peak of THz transmission significantly increases. The peak value at 0, 5, 10, − 10, − 15, and − 20 V is about 72.49, 73.39, 72.49, 79.7, 88.66, and 87.15, respectively. In order to clearly show this change, we plotted the change of device's terahertz transmission peak under different voltages in Fig. 5b. It is clear that the device only allows terahertz waves to pass under negative bias, but prevents terahertz waves from passing under positive bias. So, it is inferred that our terahertz modulator can also function as a diode for terahertz waves.
In summary, it is reported that graphene/TiO2/p-Si heterojunction can be used as a high-performance photodetector and a broadband THz wave modulator. Our proposed device has a distinct light response in the ultraviolet–visible-infrared band. The responsivity, external quantum efficiency, and detectivity are as high as 3.6 A/W, 6001%, and 4 × 1013 Jones, under 0.417 mW/cm2 density and 750 nm wavelength laser irradiation. Moreover, the transmission modulation depth of terahertz wave reaches up to 23% in the broadband of 0.3–1.0 THz at a biased voltage of − 15 V, while no any obvious change is observed in the transmission of the terahertz wave under a positive voltage, which concludes that this device can function as “a diode” relative to the terahertz wave.
Availability of data and material
All data supporting the conclusions of this article are included within the article.
Graphene-based field effect transistor
External quantum efficiency
Koppens FHL, Mueller T, Avouris P et al (2014) Photodetectors based on graphene, other two-dimensional materials and hybrid systems. Nat Nanotechnol 9:780–793
Kang P, Wang MC, Knapp PM, Nam SW (2016) Crumpled graphene photodetector with enhanced, strain-tunable, and wavelength-selective photoresponsivity. Adv Mater 28:4639–4645
Cao F, Liao Q, Deng K et al (2018) Novel perovskite/TiO2/Si trilayer heterojunctions for high-performance self-powered ultraviolet-visible-near infrared (UV-Vis-NIR) photodetectors. Nano Res 11:1722–1730
Sun H, Tian W, Cao F et al (2018) Ultrahigh-performance self-powered flexible double-twisted fibrous broadband perovskite photodetector. Adv Mater 30:1706986
Hu X, Zou P, Yin Z et al (2020) Hot-electron photodetection based on graphene transparent conductive electrode. IEEE Sens J 20:6354–6358
Wen T, Zhang D, Wen Q et al (2016) Enhanced optical modulation depth of terahertz waves by self-assembled monolayer of plasmonic gold nanoparticles. Adv Opt Mater 4:1974
Sun Z, Martinez A, Wang F (2016) Optical modulators with 2D layered materials. Nat Photonics 10:227–238
Yang DS, Jiang T, Cheng XA (2017) Optically controlled terahertz modulator by liquid-exfoliated multilayer WS2 nanosheets. Opt Express 25:16364
Qiao J, Wang S, Wang Z et al (2020) Ultrasensitive and broadband all-optically controlled THz modulator based on MoTe2/Si van der Waals heterostructure. Adv Opt Mater 8:2000160
Degl’Innocenti R, Kindness SJ, Beere HE, Ritchie DA (2018) All-integrated terahertz modulators. Nanophotonics 7:127–144
Hu M, Yan Y, Huang K et al (2018) Performance improvement of graphene/silicon photodetectors using high work function metal nanoparticles with plasma effect. Adv Opt Mater 6:1701243
Kang B, Kim Y, Yoo WJ, Lee C (2018) Ultrahigh photoresponsive device based on ReS2/graphene heterostructure. Small 14:1802593
Wei X, Yan F, Lv Q et al (2017) Fast gate-tunable photodetection in the graphene sandwiched WSe2/GaSe heterojunctions. Nanoscale 9:8388–8392
Shi YX, Li JS, Zhang L (2017) Graphene-integrated split-ring resonator terahertz modulator. Opt Quantum Electron 49:350
Chen Z, Chen X, Tao L et al (2018) Graphene controlled Brewster angle device for ultra broadband terahertz modulation. Nat Commun 9:4909
Kakenov N, Ergoktas MS, Balci O, Kocabas C (2018) Graphene based terahertz phase modulators. 2D Mater 5:035018
Wang Y, Ding K, Sun B et al (2016) Two-dimensional layered material/silicon heterojunctions for energy and optoelectronic applications. Nano Res 9:72–93
Di Bartolomeo A, Luongo G, Giubileo F et al (2017) Hybrid graphene/silicon Schottky photodiode with intrinsic gating effect. 2D Mater 4:025075
Tian W, Wang Y, Chen L, Li L (2017) Self-powered nanoscale photodetectors. Small 13:1701848
Lin S, Lu Y, Xu J et al (2017) High performance graphene/semiconductor van der Waals heterostructure optoelectronic devices. Nano Energy 40:122–148
Nair RR, Blake P, Grigorenko AN et al (2008) Fine structure constant defines visual transparency of graphene. Science 320:1308
Lv P, Zhang X, Zhang X et al (2013) High-sensitivity and fast-response graphene/crystalline silicon Schottky. IEEE Electron Device Lett 34:1337–1339
Yan F, Wei Z, Wei X et al (2018) Toward high-performance photodetectors based on 2D materials: strategy on methods. Small Methods 2:1700349
An J, Wang B, Shu C et al (2020) Research development of 2D materials based photodetectors towards mid-infrared regime. Nano Sel 2:527–540
Yu X, Li Y, Hu X et al (2018) Narrow bandgap oxide nanoparticles coupled with graphene for high performance mid-infrared photodetection. Nat Commun 9:4299
Du B, Lin L, Liu W et al (2017) Plasmonic hot electron tunneling photodetection in vertical Au-graphene hybrid nanostructures. Laser Photonics Rev 11:1600148
Shao D, Gao J, Chow P et al (2015) Organic-inorganic heterointerfaces for ultrasensitive detection of ultraviolet light. Nano Lett 15:3787–3792
Li X, Zhu M, Du M et al (2016) High detectivity graphene-silicon heterojunction photodetector. Small 12:595–601
Ma P, Salamin Y, Baeuerle B et al (2019) Plasmonically enhanced graphene photodetector featuring 100 Gbit/s data reception, high responsivity, and compact size. ACS Photonics 6:154–161
Wen QY, Tian W, Mao Q et al (2014) Graphene based all-optical spatial terahertz modulator. Sci Rep 4:7409
Sensale-Rodriguez B, Yan R, Kelly MM et al (2012) Broadband graphene terahertz modulators enabled by intraband transitions. Nat Commun 3:780
Mao Q, Wen QY, Tian W et al (2014) High-speed and broadband terahertz wave modulators based on large-area graphene field-effect transistors. Opt Lett 39:5649
Zhang D, Jin L, Wen T et al (2017) Manufacturing and terahertz wave modulation properties of graphene/Y3Fe5O12/Si hybrid nanostructures. Compos Part B Eng 111:10–16
Zhang D, Wei M, Wen T et al (2017) Infrared properties and terahertz wave modulation of graphene/MnZn ferrite/p-Si heterojunctions. Nanoscale Res Lett 12:482
Li X, Cai W, An J et al (2009) Large-area synthesis of high-quality and uniform graphene films on copper foils. Science 324:1312–1314
Li X, Zhu Y, Cai W et al (2009) Transfer of large-area graphene films for high-performance transparent conductive electrodes. Nano Lett 9:4359–4363
Ryu S, Liu L, Berciaud S et al (2010) Atmospheric oxygen binding and hole doping in deformed graphene on a SiO2 substrate. Nano Lett 10:4944–4951
Chang HC, Huang YJ, Chang HY et al (2014) Oxygen adsorption effect on nitrogen-doped graphene electrical properties. Appl Phys Express 7:055101
An X, Liu F, Jung YJ, Kar S (2013) Tunable graphene-silicon heterojunctions for ultrasensitive photodetection. Nano Lett 13:909–916
We would like to express their gratitude to EditSprings (https://www.editsprings.com/) for the expert linguistic services provided.
This work was supported by the National Natural Science Foundation of China under Grant No. 51702042, National Key Research and Development Plan under Grant No. 2016YFA0300801, National Key Scientific Instrument and Equipment Development Project No. 51827802, Sichuan Science and Technology Support Project under Grant Nos. 2021YFG0347 and 2021YFG0091.
The authors declare no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Wei, M., Zhang, D., Zhang, L. et al. High-Performance Multifunctional Photodetector and THz Modulator Based on Graphene/TiO2/p-Si Heterojunction. Nanoscale Res Lett 16, 134 (2021). https://doi.org/10.1186/s11671-021-03589-w
- Multifunctional device
- Broadband THz wave modulator